1 / 29

# Quantitative Analysis Reference Intensity Ratio (RIR) - PowerPoint PPT Presentation

Quantitative Analysis Reference Intensity Ratio (RIR). Reference Intensity Ratio (RIR) What is it?. The Reference Intensity Ratio (RIR) is a method used for Quantitative Analysis by Powder Diffraction.

I am the owner, or an agent authorized to act on behalf of the owner, of the copyrighted work described.

## PowerPoint Slideshow about ' Quantitative Analysis Reference Intensity Ratio (RIR)' - marshall-maddox

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -
Presentation Transcript
Quantitative AnalysisReference Intensity Ratio (RIR)

Reference Intensity Ratio (RIR)What is it?

The Reference Intensity Ratio (RIR) is a method used for Quantitative Analysis by Powder Diffraction.

The RIR method is based upon scaling all diffraction data to the diffraction of standard reference materials.

The intensity of a diffraction peak profile is a convolution of

many factors, only one of which is the concentration of the

analyte (species being measured).

By using the RIR method, ratios scaled to a common reference, are used in the experiment. The assumption is that all the factors, except concentration, of the analyte are ratioed and reduced to a constant.

By using ratios and measuring peak areas, the RIR method can be used to determine concentrations.

The RIR method scales all diffraction data to a standard.

By convention, corundum is used as the international reference and the scale factor is defined by:

Intensity Analyte / Intensity Corundum = I / Ic

I/Ic can be experimentally derived by adding a known weight

fraction of corundum to a pure specimen of the analyte of interest.

I/Ic can also be calculated if the atomic parameters of analyte

are known because the atomic parameters of corundum have been determined.

In PDF-4+, I/Ic has been experimentally determined for close to 10,000 materials and has been calculated for >170,000 materials.

To understand how to use I/Ic values for quantitative analysis with the PDF-4+ database, a short description of the method is provided in the following slides.

RIR

Method

RIR, as used in the Powder Diffraction File, is I/Ic (reference to corundum).

I/Ic can be determined, experimentally or calculated, from a crystal structure, both methods are used in the PDF-4+ database.

Experimentally, I/Ic can be determined by taking

the ratio of the strongest line of the pattern to the intensity of the strongest line of corundum in a 50/50 weight mixture.

If we know the crystal structure, we can calculate I/Ic as shown in the following slide.

RIR

Method

RIR

Method

All calculated patterns have I/Ic.

I/Ic = c /c c 

 = Linear attenuation coefficient

 = Absolute scale factor

 = Density

(Subscript “c” corresponds to corundum)

Single crystal determinations have all the data necessary to calculate the variables in the above equation from atomic parameters and the unit cell parameters with the use of atomic scattering factors and published constants. These are used by

the ICDD to calculate I/Ic for these entries.

RIR

Method

Calculated I/Ic values often significantly differ from

experimental I/Ic values.

Natural products, minerals, and biomaterials often contain trace impurities, anion/cation substitution in the lattice, or naturally produced vacancies, and/or defects in the crystalline state. These physical phenomena are well known to influence peak intensities and peak profiles that will change the I/c value. This value can be significantly different from one calculated from a perfect crystalline pure material.

If you are using I/Ic to quantitate a synthetic mixture, you may want to use a calculated value. If you are using I/Ic to quantitate a natural product or mineral sample, you may prefer experimental values.

Iia = intensity of reflection i of phase a

KiaXa

Iia=

a 

RIR

Method

Mainequation for quantitative analysis

Kia contains structure factor,

multiplicity, Lorentz-polarization

factor, temperature factor +

scale factor for reflection i of

phase a

Xa = wt fraction of

phase a (want this!!)

 = Linear attenuation coefficient

a is density

of phase a

Xa = wt fraction of phase a (want this!!)

KiaXa

Iia=

a 

RIR

Method

Measure this!!

KcXc

KaXa

For corundum

For analyte

Ic =

Ia=

c

a

KaXa

Ia

KaXac

Xa

Ia=

=

=

K

a

Ic

KcXca

Xc

KcXc

Ic=

c

For 50-50 mixture of analyte with corundum

Ia

=

K …..denoted (I/Ic)a

Ic

Quantitative AnalysisReference Intensity Ratios

RIR

Method

Ia

KaXac

Ia

=

=

K

=

Ic

KcXca

Ib

Ka c

Xa

Xa

Kc a

(Ia/Ic)

Xc

Xb

=

(Ib/Ic)

Kb c

Ka

Kc b

a

Kb

=

b

Quantitative AnalysisReference Intensity Ratios

RIR

Method

For any a + b mixture

Reference Intensity Ratio (RIR)Practical Considerations

RIR

Method

The RIR method uses simultaneous equations to solve analyte concentrations in a multicomponent mixture.

Many vendor programs interface to PDF-4+ to automatically extract I/Ic and peak areas from the experimental data for automated quantitative analysis.

Automated programs assume that the combination of all phases identified account for all observed scattering and 100% of the specimen. Significant errors can occur, if there are non-crystalline phases or unidentified materials present in the specimen.

Start at the main

Search Page

Go to the

Miscellaneous

Tab

1) Perform a Search

2) Select the Preferences Tab

3) Select I/Ic to display Values

TiO2’s

and I/Ic

Displayed

Choose the appropriate structure.

Many materials have polymorphs that have the same chemical formula, but different

structures. These have different I/Ic’s.

Match the reference to the specimen as closely as possible.

Use quality marks and indicators to select

the best quality reference.

Selecting I/Ic - Structure

TiO2

Rutile

I/Ic = 3.54

TiO2

Brookite

I/Ic = 3.06

Formulae are the same,

pattern, structure and I/Ic

are distinctly different

TiO2

Anatase

I/Ic = 5.04

You can select many fields that

by matching these data to the experimental data.

These include:

Chemical Name, Mineral Name

System and Space Group Number

(SG#)

Pearson, Prototype Structure and

LPF Prototype Structure

Reduced Cell, Author Cell and

Crystal Cell

Strong Line (D1, D2, D3) and

Long Line (L1, L2, L3)

From Search Results

use the Preferences Tab

to select fields

Temperature can

expand or contract

the unit cell – and

change I/Ic.

All the known factors that can alter a structure: temperature, pressure, anion or cation substitution, synthesis conditions, vacancies, stress, strain, etc. will change atom positions, electron density distribution, and therefore alter peak intensities and the I/Ic ratio.

The above factors are changes in the Kia factor in the equation for quantitative analysis.

Select a reference that most closely matches your experiment!

From the Results Form,

select Preferences,

Editor comments contain information on specimen preparation,

impurities, temperature of data collection and other factors that

can change I/Ic. They can guide you to the appropriate choice.

I/Ic for QuartzSpace Group P322175 Determinations

High Temp

Series

Data plotted from

PDF-4+ Search Form

of I/Ic versus reduced

describe T, P conditions

Ambient Data

Effect of Temp and Pressure

for Quartz I/Ic

High Pressure Series

Synthetic Materials

The database contains many quality

Indicators. These include:

Indicator High Quality Value

Quality Mark S

Status Primary

SS/FOM Highest Number

R-Factor Lowest Number

analyses conducted on the data.

The indicators are defined in the

Help documentation in the database.

Use “Preferences” to display quality marks and indicators.

Poor Quality

Low Quality Marks are designations B and O

Low Quality Status would be a “Deleted” pattern

R-factors >0.10 (i.e., 10%) and SS/FOM’s below 10 are

indications of poor quality

In general, any data meeting the above criteria should not be used in a quantitative analysis calculation as the ICDD’s editorial analysis and review would indicate that the calculation may result in large errors.

The data are included because there may not be better alternative choices for a particular material or the entry may contain other types of unique data (i.e., measured physical properties, novel synthesis, etc.).

What if a Search/Match program identified an entry with a poor quality mark or poor quality indicator?

- Check the Cross References

In this example, a Search/Match program

identified entry PDF 04-08-7810, which has

an I/Ic of 3.6 and a “B” Quality Mark. The editors’ comments mention that the atomic

parameters were derived (not experimentally

determined or calculated) from the original

publication. This results in low precision for

the cell parameters and I/Ic values.

Solution: The entry contains cross-

references identified in the “Miscellaneous

Tab” of the entry. The primary (high quality)

entry is highlighted and is an active link in

the database. The primary entry has an I/Ic of 3.61 and is an “S” quality entry.

ApplicationExamples

Using ICDD’s SIeve and SIeve+ programs, materials are identified, peak intensities of each phase are calculated and I/Ic values are displayed – allowing the user to calculate concentrations by the RIR method.

Many software distributors have RIR calculation modules, which can perform multiple, simultaneous calculations for complex mixtures, use integrated intensities and correct for absorption – all in a matter of seconds!

Examples are shown for the above.

=

Input experimental

data.

Two phase identification

in the analysis of an

unknown.

Ia

Ib

Results summary

This results in 96% magnesium aluminum silicate and

4% cerium zirconium oxide and uses peak intensities.

Automated RIR AnalysisVendor Software – Same Example

Raw Data

RIR Calculation

Difference Plot

This software calculated 92% magnesium aluminum silicate and 7% cerium zirconium oxide using integrated intensities.

Thank you for viewing our tutorial. Additional tutorials are available at the ICDD website (www.icdd.com).

International Centre for Diffraction Data

12 Campus Boulevard

Newtown Square, PA 19073

Phone: 610.325.9814

Fax: 610.325.9823